Michigan Technological University
Michigan Technological University
Digital Commons @ Michigan Tech
Digital Commons @ Michigan Tech
Michigan Tech Publications
Electronic and quantum transport properties of a graphene-BN
Electronic and quantum transport properties of a graphene-BN
Michigan Technological University, email@example.com
Michigan Technological University, firstname.lastname@example.org
Follow this and additional works at: https://digitalcommons.mtu.edu/michigantech-p
Part of the Physics Commons
Seel, M., & Pandey, R. (2018). Electronic and quantum transport properties of a graphene-BN dot-ring hetero-nanostructure. Journal of Physics Communications, 2(4), 1-9. http://dx.doi.org/10.1088/ 2399-6528/aab7df
Retrieved from: https://digitalcommons.mtu.edu/michigantech-p/399
Follow this and additional works at: https://digitalcommons.mtu.edu/michigantech-p Part of the Physics Commons
Journal of Physics Communications
PAPER • OPEN ACCESS
Electronic and quantum transport properties of a
graphene-BN dot-ring hetero-nanostructure
To cite this article: Max Seel and Ravindra Pandey 2018 J. Phys. Commun. 2 045003
View the article online for updates and enhancements.
Transport through graphene quantum dots J Güttinger, F Molitor, C Stampfer et al.
-Combined effect of oriented strain and external magnetic field on electrical properties of superlattice-graphene nanoribbons
-Perfectly conducting graphene electronic waveguide with curved channels Vahid Mosallanejad, Ke Wang, Zhenhua Qiao et al.
J. Phys. Commun.2(2018)045003 https://doi.org/10.1088/2399-6528/aab7df
Electronic and quantum transport properties of a graphene-BN
Max Seel and Ravindra Pandey
Department of Physics, Michigan Technological University, Houghton, MI 49931, United States of America
Keywords:quantum dot, quantum ring, dot-ring nanostructure, graphene, boron nitride, quantum transport, nanoelectronics
Quantum dots, quantum rings, and, most recently, quantum dot-ring nanostructures have been
studied for their interesting potential applications in nanoelectronic applications. Here, the electronic
properties of a dot-ring hetero-nanostructure consisting of a graphene ring and graphene dot with a
hexagonal boron nitride
ring serving as barrier between ring and dot are investigated using
density functional theory. Analysis of the character of the wave functions near the Fermi level and of
the charge distribution of this dot-ring structure and calculations of the quantum transport properties
nd asymmetry in the conductance resonances leading to asymmetric I
V characteristics which can
ed by applying a negative voltage potential to the central graphene dot.
Ever since the experimental discovery of graphenean immense body of theoretical and experimental work has accumulatedthat explores the unusual conduction and transport properties(for a review see for example )and possible applications in nanoelectronics and nanooptical devices. Electronic, magnetic, and optical properties of graphene quantum dots(QD)[4,5], graphene nanoribbons[6,7], and graphene quantum rings
(QR)have been analyzed. Topics include edge states in graphene rings, magneticﬁeld effects, gated rings, triangular rings, geometry effects and edge effects as obtained in tight binding and Dirac models , to name just a few. A recent example of the unusual quantum transport properties of graphene
nanostructures is a gate-voltage-tunable graphene-boron nitride(BN)resonant tunneling transistor. Growth, chemical topology, and electronic properties of a lateral graphene-BN heterostructure were investigated in aﬁrst principle study. The fabrication of graphene dots with well-deﬁned shapes remains certainly a challenge though a possible experimental realization by using carbon nanotubes as masks in an edging process has been proposed.
Recently, a novel nanostructure that consists of a quantum dot surrounded by a quantum ring with a potential barrier between these parts was proposed and its transport properties have been investigated[16,17]. It was shown that the wave function of this dot-ring nanostructure(DRN)can be shifted from the dot to the ring by tuning the position of the QD potential which can be realized by an appropriate gate voltage applied to the central dot part.
In this paper we now explore whether a DRN can be realized by using a graphene ring, an inner graphene dot, and a hexagonal boron nitride(h-BN)ring serving as barrier between outer graphene ring and central dot. The
nanostructure for whichﬁrst principle calculations are performed is shown inﬁgure1. After an analysis of the energy level structure of this graphene-h-BN DRN, of the charge distribution and the electrostatic potential, quantum transport properties are investigated. It is found that asymmetry in the conductance resonances leads to asymmetric I–V characteristics which can be modiﬁed by applying a negative voltage potential to the central graphene dot.
2. Method and computational details
The graphene-h-BN dot-ring hetero-nanostructure consists of an outer ring with 168 C atoms and zigzag edges, an inner dot with 96 C atoms, and a BN ring with 60 B and 60 N atoms(seeﬁgure1). The dangling bonds at the
OPEN ACCESS RECEIVED
1 November 2017
9 March 2018
ACCEPTED FOR PUBLICATION
19 March 2018
3 April 2018
Original content from this work may be used under the terms of theCreative Commons Attribution 3.0 licence.
Any further distribution of this work must maintain attribution to the author(s)and the title of the work, journal citation and DOI.
edges are passivated with 48 H atoms to ensure that each boundary carbon atom has the correct number of neighbors simulating sp2bonding character. The DRN consists of a total of 432 atoms and has a diameter of 37 Å. Calculations were also performed for the individual parts of the system, i.e., for the C188H84 ring, the B60N60H60 ring, and for the C96H24 inner dot(the number of H atoms is determined by the number of edge atoms).
All calculations were performed with GAUSSIAN09using density functional theory(DFT)with Becke’s 3-parameter hybrid functional B3LYPwith non-local correlation provided by the Lee, Yang, and Parr(LYP) expression. Since in this exploratory study we are only interested in basic trends and not absolute quantitative numbers, the experimental values of the bond lengths for graphene and BN monolayer were used. No geometry optimization was performed. The 6-31 basis set instead of the more commonly employed 6-31(d,p)basis set was used(the B3LYP 6-31(d,p)level of theory has become a standard for a reasonable balance between accuracy and computer time for larger systems when compared to available experimental data). A direct comparison of 6-31 and 6-31(d,p)basis sets results for C96H24(912 versus 1560 basis functions)shows that the gap between the highest occupied(HOMO)and lowest unoccupied molecular orbital(LUMO)of the graphene dot changes only from 1.95 eV to 1.93 eV with no qualitative differences in the the nature of the wave functions or charge density population. Using the 6-31 basis set the DRN system with 432 atoms has 3552 basis functions. A more detailed discussion of B3LYP results for graphene quantum dots, comparison to available experimental data, and insights gained from electronic structure calculations can be found in.
To demonstrate possible applications of the proposed dot-ring hetero-structure in nanoelectronic devices we compute its quantum transport properties in the tight binding approximation using the open software package Kwant. The program package Kwant provides an easy way for exploratory calculations to compute the conductance using the Landauer-Büttiker formalism[23,24]. For the tight binding Hamiltonian in theﬁrst neighbor approximation
= ∣ñá +∣ ∣ñá∣ ( )
H u i ii t i jij 1
where i and j label nearest neighbor sites on a hexagonal lattice, we chose uC=0 eV, uN=−1.0 eV, and
uB=3.6 eV for the onsite parameters[25,26]and the same hopping parameter tij=t=−2.7 eV for allﬁrst
neighbor interactions. It is not to be expected that taking into account more neighbors interactions or moreﬁ ne-tuned hopping parameters(e.g. tBN=−2.5 eV, tCN=−2.3 eV, tCB=−2.1 eV)will change the qualitative
features of the quantum transport results. Earlier tight binding resultsfor quantum transport in graphene– boron nitride lateral heterostructures corroborate the importance of the sign difference in the on-site parameters for N and B in the lattice and the robustness of the results with regard to small changes in the hopping
Kwant also allows easily to take into account the effect of a magneticﬁeld by using Peierls substitution [27,28]to include a vector potentialÂ=(−B.y, 0, 0)in the hopping parameter(Landau gauge for a constant
Figure 1.The graphene-BN dot-ring hetero-nanostructure with a diameter of 37 Å: an outer ring with 168 C atoms(grey), an inner dot with 96 C atoms, a BN ring with 60 B(pink)and 60 N(blue)atoms, and 48 H atoms(white)to passivate the dangling bonds of the carbon edge atoms.
perpendicular magneticﬁeld B in z-direction and leads in the x-direction)
F = - F - +
( / ) [ / ( )( )/ ] ( )
tij 0 t exp i 0 xi xj yi yj 2 2
withΦ0=h/e being the magneticﬂux quantum. To benchmark our results, we checked our adaption of Kwant
by reproducing the 2n+1 dependence(n=0, 1, 2,.)for the dimensionless quantum conductance
(expressed in the unit of quantum conductance 2 e2/h)and the unconventional quantum Hall effectfor the graphene zigzag nanoribbons used as leads to the DRN. Figure2(a)shows the graphene nanoribbon with a width of∼8 a(a=2.46 Å is the graphene lattice constant)used later as lead, the location at E=0 of the degenerate zigzag edge state(ﬁgure2(b))which provides the conduction channel(ﬁgure2(c))in the energy region later discussed.
Metallic leads are needed for calculations of electronic transport. Zigzag nano ribbons were chosen because they are always metallic due to the edge state and therefore provide a conduction channel at the Fermi energy E=0, whereas armchair ribbons are semiconducting or, depending on the width, metallic with vanishing DOS at E=0. On the other hand, quantum dots with armchair edges have larger bandgaps, so overall, one would expect an electronic structure with fewer states(or no states in the case of armchair ribbons as leads)in the region of interest that contribute to the transport properties.
3. Results and discussion
3.1. Electronic properties
The electronic properties of the DRN are determined by the energy spectrum and the wavefunctions nearest to the Fermi energy. The B3LYP-DFT/6-31G results are summarized inﬁgure3. To analyze the spectrum of the DRN it is helpful to look into the energy level diagram of the(non-interacting)constituent parts: the outer C168 ring(gap EG=1.25 eV), the BN120 ring constituting a barrier(EG=6.11 eV), and the C96 dot(EG=1.95 eV).
Figure 2.(a)Zigzag graphene nanoribbon with 9 unit cells; black and white circles indicate the AB sublattices of graphene; width
∼20 Å(x andyaxis are in units of the graphene lattice constant a=2.46 Å); fading red indicates continuation to inﬁnity(b)Band structure of this nanoribbon with 9 valence and conduction subbands; the localized edge states become degenerate at the Fermi level EF=0 between k=4π/3 3andπ.(c)Conductance of this nanoribbon(in units of 2e2/h to account for the spin degeneracy of each subband); it increases as 2n+1, n=0, 1, 2,Kuntil the maximum 9(=number of subbands)is reached at E=|t|=2.7 eV.
The positions of the energy levels of the highest occupied and lowest unoccupied MOs of these constituent parts deﬁne a single particle well structure where the potential energy bottom of the ring is(1.95−1.25)/2 eV=0.35 eV below the bottom of the central dot separated by a barrier of(6.11−1.25)/2 eV=2.43 eV due to the BN ring. It is therefore to be expected that the wavefunctions nearest to the Fermi energy EFwill be conﬁned to the outer ring. This
is also not surprising because the zigzag edge states of a graphene structure are always nearest to EF.
When the interaction between these constituent parts is turned on, that is, the electronic properties of the DRN as shown inﬁgure1are calculated, the gap is reduced to 0.77 eV, which is only slightly larger than the 0.65 eV gap obtained for the corresponding C384H48 graphene quantum dot. The highest occupied and lowest unoccupied MOs are shown inﬁgure4. As expected from the nature of the well structure, the doubly degenerate HOMO and LUMO orbitals are conﬁned to the outer ring as is the HOMO-1 and LUMO+1 state. The doubly degenerate HOMO-2 and the LUMO+2 orbitals are theﬁrst wavefunctions that are mainly conﬁned to the inner dot. Due to the twofold degeneracy of the HOMO and LUMO orbitals, each orbital alone does not reﬂect the symmetry with respect to 2π/3 rotation about its center but a linear combination of these would. The non-degenerate HOMO-1 and LUMO+1 clearly reﬂect the symmetry.
A Mulliken population analysis reveals that signiﬁcant charge transfer occurs within the DRN, the main feature being a positively charged inner quantum dot and a negatively charged BN barrier: the C96 dot has a net charge of+2.6 e, the BN ring carries a charge of−6.4 e, the outer C168 ring−2.6 e, and the passivating 48 H atoms+6.4 e. A more detailed and better picture of the charge distribution within the DRN can be seen in the electrostatic potential(ESP)map given inﬁgure5: shades of blue indicate relative absence of electrons(around the B atoms)and red relative abundance of electrons(around N and sets of C atoms). It is to be expected that the distribution of positive and negative charges in different regions of the DRN and the conﬁnement of different orbitals near the Fermi energy either in the outer ring or inner dot lead to novel transport properties different from those of a regular graphene quantum dot. This will be explored in the next section by calculating quantum transport properties using a tight binding model.
3.2. Quantum transport properties
In order to explore the transport properties of a dot-ring nanostructure consisting of graphene and h-BN we used the tight binding Hamiltonian described in section2and the software package Kwant. The results are summarized inﬁgure6.
Figure 3.Molecular Orbital energy level diagram of the DRN compared to the(non-interacting)constituent parts: the outer C168 ring
(EG=1.25 eV), the BN120 ring barrier(EG=6.11 eV), and the C96 dot(EG=1.95 eV). Due to symmetry, all HOMO and LUMO orbitals are doubly degenerate. The structures are aligned with the gap midpoint deﬁned as EF=0. Only energy levels close to EFare shown. The width of the ring, barrier, and dot corresponding to a cross section of the DRN is indicated in Å.
The DRN is shown inﬁgure6(a). It has a diameter of∼50 Å(20 a with a=2.46 Å being the lattice parameter of graphene). The width of the graphene ribbon leads is∼20 Å. A narrow BN barrier ring separates the inner dot with a diameter of∼25 Å from the outer graphene ring. An analysis of the tight binding wavefunctions around EF
shows that they are again-as found before in theﬁrst principle study-localized in the outer ring.
The tight binding structure represents a larger, more rounded structure(∼50 Å diameter)than theab inito one(hexagon diameter∼37 Å). It also has a mix of zigzag and armchair edges. Passivating H atoms at the edge atoms are not necessary because each atom is assumed to contribute oneπorbital, each atom has the same on-site parameter independent of its location. Despite the differences, an analysis of the eigenvalues and eigenvectors around the Fermi energy reveals qualitatively similar properties: the tight binding wave functions corresponding to eigenvalues immediately around EFare again localized in the outer ring, followed by
eigenvalues and wavefunctions localized in the inner dot, i.e., they show the properties desired for a dot-ring nanostructure. One can therefore expect, that the transport properties found for the tight binding structure will describe(at least qualitatively)the properties expected from a fullab initotransport calculation for the hexagonal structure.
To benchmark the DRN results, weﬁrst compute the conductance of the corresponding graphene dot with a diameter of 50 Å.(seeﬁgure6(b). It shows the expected structure with resonances symmetric around EF=0.
The peak maximum is deﬁned by the conductance value of the graphene ribbon in this energy range which is at theﬁrst plateau of 2 e2/h(seeﬁgure2(c). The conductance of the DRN is shown inﬁgure6(c). It shows a slightly
Figure 4.Highest occupied and lowest unoccupied molecular orbitals of the dot-ring nanostructure depicted inﬁgure1. The doubly degenerate HOMO and LUMO orbitals are conﬁned to the outer ring as is the HOMO-1 and LUMO+1 state. The doubly degenerate HOMO-2 and the LUMO+2 orbitals are theﬁrst wavefunctions that are mainly conﬁned to the inner dot.
narrower peak structure and is asymmetric around EF=0 with smaller transmission probabilities in the
positive energy range.
In the tight binding model a gate voltage or a p-n junction can simply be modeled by adding to the on-site parameters uia potential±UGfor p(n)regions[22,30]. Therefore, to model a negative gate potential applied to
the inner dot the on-site energy of the inner-dot C atoms is modiﬁed by UG=−0.5 eV. The resulting
conductance is shown inﬁgure6(d). The negative gate voltage increases the transmission probability in the positive energy range with a new resonance peak emerging at∼+0.3 eV. The states associated with this new resonance are two wavefunctions mainly localized on the inner dot: they are pulled down from∼0.7 eV, the corresponding eigenvalue of the DRN without applied gate voltage. A positive gate voltage of UG=+0.5 eV
pushes these two eigenvalues to 0.75 and 0.79 eV and the associated wavefunctions are localized on the ring, not on the inner dot.
The current can be calculated by using the Landauer formula[23,31]
ò= --¥ ¥ ( )[ ] ( ) I 2e f h T E L fR dE 3
T(E)is the transmission function, fL(fR)the Fermi–Dirac distribution for the left(right)lead. For low
temperatures, the upper limit can be approximated by the Fermi energyEFL(E )
FR with fL(fR)=1 in the
respective integration regions so that the integral becomes
òD T E dE( )
ifEFLis shifted by+Δand
-D T E dE( )
when shifted by−Δ(Δin eV;EFRkept at 0). The relation between the transmission function T(E)and conductance G(E)plotted before is
Figure 5.The electrostatic potential(ESP)map of the DRN shown inﬁgure1. Shades of blue(red)indicate relative absence
Figure 6.(a)Geometry of the DRN with an outer ring radius of 10 a(x andyaxis are in units of the graphene lattice constant a=2.46 Å), a second ring with radius of 7 a, and an inner dot radius of 5 a. The width of the leads is 8 a. N atoms are green, B atoms grey, C atoms brown. Fading red indicates continuation to inﬁnity.(b)Conductance of a graphene dot with resonances symmetric around EF=0.(c)Conductance of the DRN.(d)Conductance of the DRN when the on-site energy of the C atoms of the inner dot is modiﬁed by UG=−0.5 eV to model a negative gate potential applied to the inner dot.
( ) / ( ) ( )
G E 2e2 hT E . 4
With 2e2/h=7.75×10−5[Ω−1], the resulting currents are plotted inﬁgure7.
For the graphene dot the conductance with resonances symmetric around EF=0(seeﬁgure6(b))leads to a
current increase from−20μA to+20μA symmetric around 0 when the bias voltage changes from−0.6 V to +0.6 V(blue curve inﬁgure7(a)). Sections of steeper increases followed byﬂatter or plateau-like segments approximate a straight line with an overall slope ofΔI/ΔV∼20μA/0.6 V∼33μA/V. For comparison we show the I–V characteristics of the graphene zigzag ribbon inﬁgure7(b): since between−0.6 eV and+0.6 eV its conductance has a constant value of 2e2/h(seeﬁgure2(c); the zigzag edge state provides the only conduction channel)the current increases linearly with a slope ofΔI/ΔV∼45μA/0.6 V∼75μA/V corresponding to a resistivity of∼13 kΩ. The order of magnitude is consistent with experimental resultsthat show that the resistivity of a ribbon increases as the width decreases with a resistivity between 10–15 kΩfor a ribbon width around 20 nm.
For the DRN, the plateaus in the I–V curve are more pronounced compared to the graphene dot due to the sharper peak structure in the conductance(seeﬁgure6(c)), but the noticeable difference is the asymmetry between a negative and positive applied voltage resembling the IV characteristics of a n-p junction: between
−0.6 V and zero the current changes from−10μA to zero, then it stays zero until∼0.2 V toﬁnally reach a value of only∼2μA, 5 times smaller than that for a negative voltage and 10 times smaller than the current found for the graphene dot. When the gate potential of−0.5 eV is applied to the inner dot(red curve inﬁgure7(a))the asymmetry is partially lifted: for positive voltage, the current is still zero until∼0.2 V but then increases to a value of∼7μA for 0.6 V, comparable to the value of approximately−8μA at−0.6 V. For a positive gate potential of +0.5 eV(green curve inﬁgure7(a))the asymmetry persists and the conductance resembles the conductance of the DRN with zero gate voltage.
4. Summary and conclusion
In summary, we have analyzed the electronic and quantum conduction properties of a novel quantum dot-ring nanostructure consisting of an outer graphene ring separated from an inner graphene quantum dot by a BN ring serving as barrier. The distribution of positive and negative charges in different regions of the DRN and the conﬁnement of orbitals near the Fermi energy either in the outer ring or inner dot obtained fromﬁrst principle calculations suggests tunable conduction properties. Exploratory tight binding quantum transport calculations show that asymmetry in the conductance resonances of the DRN leads to asymmetric I–V characteristics which can be modiﬁed by applying a negative voltage potential to the central graphene dot and have dot wave functions contributing to the conductance.
Dot-ring nanostructures can be fabricatedby cutting a slice of a core–shell nanowire with a potential barrier between the core and the shell. The dimensions of experimentally fabricated heterostructures are certainly larger. Here, for an exploratory calculation, the dimensions of the quantum dot-ring structure were chosen to allow for reasonable computer times. For a larger ring-dot structure which might be experimentally feasible, we would still expect that the mechanism responsible for the transport properties, i.e., the shifting of the dot wave function to allow for a resonance with the ring and lead wave function, will hold.
Figure 7.(a)I–V characteristics of the DRN without(black)and with an applied gate voltage(red and green)at the central dot compared to a graphene dot(blue).(b)I–V characteristics of a graphene dot(blue)compared to the graphene ribbon leads(green).
Helpful discussions with Gaoxue Wang and Kevin Waters are gratefully acknowledged. The generous support with computer time by Michigan Tech’s High Performance Computer Center is very much appreciated.
Max Seel https://orcid.org/0000-0002-1535-9900 Ravindra Pandey https://orcid.org/0000-0002-2126-1985
Novoselov K S, Geim A K, Morozov S V, Jiang D, Zhang Y, Dubonos S V, Grigorieva I V and Firsov A A 2004Science306666–9 Geim A K and Novoselov K S 2007Nature Mat.6183–91
Stampfer Cet al2011Front. Phys.6271–93
Sun H, Wu L, Wei W and Qu X 2013Materials Today16433–42 Lee Jet al2016Nature Physics121032–6
Zhong X, Pandey R and Karna S P 2012Carbon50784
Wakabayashi K, Sasaki K, Nakanishi T and Enoki T 2010Sci Technol Adv Mater11054504
Fomin V M(ed)2014Physics of Quantum Rings, Nano Science and Technology(Berlin Heidelberg: Springer) Bahamon D A, Pereira A L C and Schulz P A 2009Phys. Rev.B79125414
Wurm J, Wimmer M, Baranger H U and Richter K 2010Semicond. Sci. Technol.25034003 Potasz P, Guclu A D and Hawrylak P 2010Phys. Rev.B82075425
Potasz P, Guclu A D, Voznyy O, Folk J A and Hawrylak P 2011Phys. Rev.B83174441
da Costa D R, Chaves A, Zarenia M, Pereira J M Jr, Farias G A and Peeters F M 2014Phys. Rev.B89075418
Britnell L, Gorbachev R V, Geim A K, Ponomarenko L A, Mishchenko A, Greenaway M T, Fromhold T M, Novoselov K S and Eaves L 2013Nature Communications.41794
Loh G C and Pandey R 2015J. Mater. Chem.C35918–32
Zipper E, Kurpas M and Maska M M 2012New Journal of Physics14093029
Janus-Zygmunt I, Kedzierska B, Gorczyca-Goraj A, Zipper E and Maska M M 2016International Journal of Modern PhysicsB30 1642013
Frisch M Jet al2009Gaussian 09, Revision D.01(Wallingford CT: Gaussian, Inc.) Becke A D 1993J. Chem. Phys.985648–52
Lee C, Yang W and Parr R G 1988Phys RevB37785–9 Schumacher S 2011Phys. Rev.B83081417
Groth C W, Wimmer M, Akhmerov A R and Waintal X 2014New J. Phys.16063065see also:(https://kwant-project.org/) Landauer R 1957IBM J. Res. Dev.1223
Landauer R 1988IBM J. Res. Dev.32306and references therein Büttiker M 1986Phys. Rev. Lett.571761
Jungthawan S, Limpijumnong S and Kuo J L 2011Phys. Rev.B84235424 Abergel D S L 2016J. Phys.: Condens. Matter29075303
Peierls R E 1933Z. Phys80763 Hofstadter D R 1976Phys. Rev.B142239
Gusynin V P and Sharapov S G 2005Phys. Rev. Lett.95146801
Zarenia M, Pereira J M Jr, Peeters F M and Farias G A 2013Phys. Rev.B87035426
Curevas J C and Scheer E 2010Molecular Electronics : An Introduction to Theory and Experiment(Singapore: World Scientiﬁc)
Chen Z, Lin Y M, Rooks M J and Avouris P 2007Physica.E40228-232 Lauhon L J, Gudiksen M S, Wang D and Lieber C M 2002Nature42057–61